week ending 17 MAY 2013

PHYSICAL REVIEW LETTERS

Thermal Phase Transitions in Artificial Spin Ice Demian Levis,1 Leticia F. Cugliandolo,1 Laura Foini,1 and Marco Tarzia2 1

Universite´ Pierre et Marie Curie-Paris 6, Laboratoire de Physique The´orique et Hautes Energies, 4, Place Jussieu, Tour 13, 5e`me e´tage, 75252 Paris Cedex 05, France 2 Universite´ Pierre et Marie Curie-Paris 6, Laboratoire de Physique The´orique de la Matie`re Condense´e, 4, Place Jussieu, Tour 12, 5e`me e´tage, 75252 Paris Cedex 05, France (Received 15 February 2013; published 14 May 2013) We use the sixteen-vertex model to describe bidimensional artificial spin ice. We find excellent agreement between vertex densities in 15 differently grown samples and the predictions of the model. Our results demonstrate that the samples are in usual thermal equilibrium away from a critical point separating a disordered and an antiferromagnetic phase in the model. The second-order phase transition that we predict suggests that the spatial arrangement of vertices in near-critical artificial spin ice should be studied in more detail in order to verify whether they show the expected space and time long-range correlations. DOI: 10.1103/PhysRevLett.110.207206

PACS numbers: 75.10.Hk, 05.70.Jk, 05.70.Ln, 75.50.Lk

Hard local constraints produce a rich variety of collective behavior such as the splitting of phase space into different topological sectors and the existence of ‘‘topological phases’’ that cannot be described with conventional order parameters [1]. In geometrically constrained magnets, the local minimization of the interaction energy on a frustrated unit gives rise to a macroscopic degeneracy of the ground state [2], unconventional phase transitions [3,4], the emergence of a Coulomb phase with long-range correlations [5,6], and slow dynamics [7,8] in both 2D and 3D systems. In this work we focus on a paradigm with these features: spin ice, a class of magnets frustrated by the ice rules [9–11]. In natural spin ice the ice rules are due to two facts: the pyrochlore lattice structure, in which magnetic ions sit on the vertices of corner sharing tetrahedra, and the ferromagnetic interaction between the Ising-like moments that are forced to lie on the edges joining the centers of neighboring tetrahedra. The energy of each unit cell is thus minimized by configurations with two spins pointing in and two pointing out of the center of the cell. All configurations satisfying the local constraint are degenerate ground states if the ice-rule preserving vertices are equally probable. This is the same mechanism whereby water ice has a nonvanishing zero-point entropy that is, indeed, remarkably close to the one of the Dy2 Ti2 O7 spin-ice compound [12]. These materials received renewed interest in recent years when a formal mapping to magnetostatics suggested to interpret the local configurations violating the spin-ice rule as magnetic charges [13]. However, detailed study of such defects in 3D remains a hard experimental task. Two-dimensional Ising-like ice models had no experimental counterpart until recently when it became possible to manufacture artificial samples made of arrays of elongated single-domain ferromagnetic nanoislands frustrated by dipolar interactions. The beauty of artificial spin ice 0031-9007=13=110(20)=207206(5)

(ASI) is that the interaction parameters can be precisely engineered—by tuning the distance between islands, i.e., the lattice constant, or by applying external fields—and the microstates can be directly imaged with magnetic force microscopy (MFM) [14], photoemission electron microscopy [15], or Lorentz transmission electron microscopy [16]. These systems should set into different phases depending on the experimental conditions [17]. However, the lack of thermal fluctuations due to the high energy barriers for single spin flips had prevented the observation of the expected twofold degenerate antiferromagnetic (AFM) ground state. Recently, these problems have been partially overcome via (i) the gradual magnetofluidization of an initially polarized state [18] and (ii) the thermalization of the system during the slow growth of the samples [19]. Although with demagnetization the actual AFM state of square ASI was never reached, the statistical study of a large number of frozen configurations of samples with up to 106 vertices at interaction-dominated low energies became possible [18]. With the procedure proposed in (ii), large regions with AFM order were formed in a few samples when sufficiently small lattice constant and weak disorder were used. Whether the sampling of a conventional thermal equilibrium ensemble is achieved in this way is a question that was raised in [19,20] and that we will address here. The purpose of this Letter is to interpret and explain recent experimental observations on ASI [18–20]. We consider a simple schematic model for 2D dipolar spin ice, the sixteen-vertex model (see Fig. 1) [4,8], where dipolar interactions beyond nearest-neighbor vertices are neglected. We compare the equilibrium and out-ofequilibrium properties of the model with the experimental results and we match the behavior of several observables (such as the densities of different vertex types hni i) with data on ASI samples [19,20]. This approach is at face value

207206-1

Ó 2013 American Physical Society

PRL 110, 207206 (2013)

PHYSICAL REVIEW LETTERS

FIG. 1 (color online). Top: Sixteen vertex configurations and their statistical weights !i / expði Þ. The first six vertices, v1 ; . . . ; v6 , satisfy the ice rule and have vanishing magnetic charge. Vertices v1 ; . . . ; v4 carry a dipolar moment while v5 and v6 do not. The last ten vertices are ‘‘defects’’: v7 and v8 have magnetic charge 4 and no dipole moment while v9 ; . . . ; v16 have magnetic charge 2 and a net dipole moment. Bottom: Ground state configurations of the model. (a) Paramagnetic (PM) state, (b) c-AFM order, (c) a-FM order.

similar but actually very different from the one used in previous studies [18,20], where data were fitted in terms of single independent vertices (with no topological interactions), as hni i / expðeff i Þ, with the effective temperature eff introduced as a fitting parameter. In our approach frustrated interactions are fully taken into account. We address the issue of thermalization of ASI samples and we make several predictions that could be tested in the lab. The samples and the model.—In their simplest setting ASI are 2D arrays of elongated single-domain permalloy islands whose shape anisotropy defines Ising-like spins arranged along the edges of a regular square lattice. Spins interact through dipolar exchanges and the dominant contributions are the ones between neighboring islands across a given vertex. No configuration of the surrounding spins can minimize all pairwise dipole-dipole interactions on a vertex. In samples with no height offset (h ¼ 0), 2D square symmetry defines four relevant vertex types of increasing energy, where the c vertices take the lowest value, leading to a ground state with staggered c-AFM order (see Fig. 1). Note that the relative energies of the different vertex configurations could be tuned by h in such a way that the ground state displayed ferromagnetic (FM) order [17] as depicted in Fig. 1(c). We mimic the experimental samples with the sixteenvertex model defined as follows: Ising spins sit along the edges of an L L square lattice. Long-range interactions beyond next-nearest-neighbor spins are neglected and the magnetostatic energies i of the sixteen vertex configurations are attributed as explained above. The total energy is givenPin terms of populations ni of distinct vertex types, E ¼ 16 i¼1 ni i . Despite the simple form of E, nontrivial frustrated topological interactions between vertices are

week ending 17 MAY 2013

present as each pair of neighboring vertices shares one spin. The model is coupled to a thermal bath at inverse temperature . We introduce the statistical weights !i / expði Þ, that in the vertex models’ literature are referred to as a ¼ !1 ¼ !2 , b ¼ !3 ¼ !4 , c ¼ !5 ¼ !6 , d ¼ !7 ¼ !8 , and e ¼ !9 ¼ ¼ !16 [4] (see Fig. 1). The equilibrium properties can thus be described in terms of four different statistical weights satisfying c > ða ¼ bÞ > e > d. We study the equilibrium and out-of-equilibrium properties of the sixteen-vertex model in two ways. We perform numerical simulations of the 2D model with a single spin flip Monte Carlo (MC) algorithm improved with the rejection-free continuous time setup (CTMC). We also employ an analytic approach put forward in [21], based on a sophisticated version of a cluster variational meanfield Bethe-Peierls (CVBP) formalism, by defining the model on a coordination-four tree made of square plaquettes (an extension over a tree of single vertices is necessary to describe an AFM phase populated by finite loop fluctuations). Details of this method have been extensively reported in [21], where the phase diagram was derived for generic values of the ratios a=c, b=c, d=c, e=c, showing that the CVBP technique describes with very good accuracy the equilibrium properties as compared to MC simulations. Density of vertices.—In the experiments in [19,20] the thickness of the magnetic islands grows by deposition (at constant temperature and all other external parameters within experimental accuracy) on 15 lattices with five different lattice constants and using three material underlayers (Si, Ti, Cr) in each of them. (We refer to the Supplemental Material in [20] for more details on the parameters and materials used.) The Ising spins flip by thermal fluctuations during the growth process. However, as the energy barrier for single spin flips increases with the size of the islands, once a certain thickness is reached the barrier crosses over the thermal fluctuations of the bath, kB T, and the spins freeze. At the end of the growth process, the spin configurations are imaged with MFM and the number of vertices of each kind are counted on five independent square areas with, roughly, 27 27 vertices each. Average values (and statistical errors) are also estimated. Our analysis is as follows. For each set of vertex concentrations measured in [20] at a given lattice constant, we determine the statistical weights c, a, e, and d—and thus c , a , e , and d —that better match the data, by solving the sixteen-vertex model with the CVBP approximation and imposing P n eH ða;c;d;eÞ hni iexpt ¼ hni iCVBP ¼ PC i H ða;c;d;eÞ ; (1) Ce where the sum runs over all possible vertex configurations C. Surprisingly enough, it turns out that the energy ratios are approximatively constant within the statistical errors

207206-2

PRL 110, 207206 (2013)

week ending 17 MAY 2013

PHYSICAL REVIEW LETTERS

for almost all the lattice spacings of the as-grown samples, and coincide with the values used by Nisoli et al. [18]. Such energy ratios can be rationalized in terms of magnetostatic exchanges due to dipolar interactions. More precisely, if each dipole is modeled as a pair of oppositely charged monopoles and Coulomb interactions between monopoles around a single vertex pﬃﬃﬃ are only taken into account, p one ﬃﬃﬃ finds c ¼ 2ð1 2 2Þ=‘, a ¼ 2=‘, e ¼ 0, d ¼ 2ð2 2 þ 1Þ=‘ (‘ being the lattice constant). As a consequence, the statistical weights can be expressed in term of a single energy scale 0 as c ¼ 1, a ¼ e0 , e ¼ , with ere 0 , and d ¼ erd 0 p ﬃﬃﬃ the energy pﬃﬃﬃ ratios re and rd being p equal to r ¼ ð2 2 1Þ=ð2 2 2Þ ’ 2:207 and ﬃﬃﬃ pﬃﬃﬃ e rd ¼ 2 2=ð 2 1Þ ’ 6:828. Remarkably, no fitting parameter nor effective temperature has to be introduced to describe the data: is the true inverse temperature at which experiments are performed and 0 is an energy scale that only depends on ‘ and the underlayer, and which could be in principle determined from a microscopic calculation. In Fig. 2 we plot the thermal averages of the vertex densities as a function of the energy scale 0 . The CTMC results (hni isim , empty symbols) and CVBP calculations (hni iCVBP , solid lines) are in excellent agreement. They show a second-order phase transition from a paramagnetic (PM) phase at low to an AFM phase dominated by type-c vertices at high , where both translational invariance and spin reversal symmetry are spontaneously broken. We also include data from [20] (full symbols) that are in remarkably good agreement with the sixteen-vertex model curves (except for a few points that turn out to be quite close to the critical temperature). Such a good accord confirms that dipolar interactions beyond nearest-neighbor vertices do not play a prominent role and that the sixteen-vertex model mimics ASI samples. It also points out that the simple picture in [18] provides a good estimate of the energy ratios between 1 0.8 nc na b ne nd

ni

0.6 0.4

different vertex types. Most importantly, these results strongly suggest that as-grown artificial spin-ices studied in [19,20] sample the conventional thermal equilibrium ensemble for most experimental points. Phases and phase transition.—We focus now on the PMAFM phase transition. In Fig. 3 we present equilibrium CTMC data for [Fig. 3(a)] the order parameter describing c-AFM ordering, M ¼ 12 ðhjmx ji þ hjmy jiÞ, where mx;y are the staggered magnetizations along the horizontal and vertical directions, and [Fig. 3(b)] the heat capacity C ¼ L2 ðhE2 i hEi2 Þ as a function of the distance to the critical inverse temperature, ð c Þ=c . The data clearly show the presence of a second-order phase transition from a PM phase to a c-AFM phase as is increased above c . The analytic results (shown with solid red lines) show a systematic shift of the critical point by about 10% towards higher temperature, as expected for mean-field ¼ 1:05 and sim calculations. We find CVBP c c ¼ 1:2, where here and in the following we measure in units of 0 . We determine c ¼ 1:204 0:008 independently with a nonequilibrium relaxation method [22], by identifying c as the inverse temperature at which the staggered magnetization decays algebraically, M ðtÞ t=ðzc Þ , where and are the equilibrium order parameter and correlation length critical exponents, respectively, and zc is the dynamical exponent. Away from c an exponential decay is instead observed. This confirms that the criticality of the spin liquid phase [4,23] is broken by the presence of defects at finite temperature. Previous numerical studies predict thermodynamic transitions in the model with dipolar interactions as well [17,24]. Correlation functions.—Stochastic thermal evolution and canonical equilibration not only yield the vertex densities but also the correlation functions. Figure 4(a) shows the space dependence of the two-point function Cðr; tÞ ¼ P L2 h i;j Si;j ðtÞSiþr;jþr ðtÞi at different times after a quench from ¼ 0 to c ¼ 1:2. Si;j denote the spins sitting along the edges of the L L square lattice, with Si;j ¼ þ1 if the spin points right or up and Si;j ¼ 1 otherwise. r is pﬃﬃﬃ measured in units of ‘= 2. These data have been averaged over 103 independent runs of a system with L ¼ 60. At large times the curves approach the equilibrium asymptotic

0.2 0 0

0.5

1

1.5

2

(a)

(b)

0

FIG. 2 (color online). Average densities of different vertex types as a function of 0 . Full symbols with error bars are experimental data [20], hni iexpt . Empty symbols with dotted lines correspond to the equilibrium CTMC data, hni isim . The CVBP analytic solution, hni iCVBP , of the sixteen-vertex model is shown in solid lines.

FIG. 3 (color online). Staggered magnetization M (a) and specific heat C (b) as a function of the distance to the inverse critical temperature c for system sizes L ¼ 30, 40, 50, 60. The (red) solid lines are the results of the CVBP analytic calculation.

207206-3

PRL 110, 207206 (2013)

coarsening process if the initial condition is a disordered high temperature one. In equilibrium correlations decay 2 exponentially, Cðr; t ! 1Þ A expðr=Þ þ M (dotted 2 black line). The asymptotic value M 0:73 is consistent with the data shown in Fig. 3, and the correlation length is ð ¼ 1:36Þ 3. On the other hand, out-of-equilibrium spatial correlations decay to zero at large distances. The data for Cðr; tÞ collapse onto a single curve when the length variable r is rescaled by t1=2 (see the inset). This scaling is accurate in the coarsening regime only: it fails at times larger than 2600 MC simulations and smaller than 100 MC simulations. The snapshots in Fig. 5 and the t1=2 scaling strongly suggest that the coarsening dynamics is curvature driven [26]. These results imply that the samples obtained by using the rotating field protocol [18], where no correlations beyond first neighbors were observed, have not achieved equilibrium. On the contrary, the as-grown samples in [19,20] are likely to be near equilibrium. However, as also shown by our numerical results, close to the phase transition critical slowing down sets in, and in the whole AFM phase slow coarsening dynamics emerge. It remains therefore to be understood whether critical and subcritical samples have fully equilibrated. To settle this issue one should grow samples with a slower deposition rate and measure, if possible, time-dependent observables during growth (such as the staggered magnetization and two-times

(a) (b) × ×

FIG. 4 (color online). Space-time correlations Cðr; tÞ after a quench from ¼ 0 to c 1:2 (a) and ¼ 1:36 (b), in a system with L ¼ 60. The colored lines and points are data taken at different times. The dotted black lines are the t ! 1 equilibrium functions, Cðr; t ! 1Þ r2þd , with ¼ 1=4, and 2 , with M2 0:73, 3. Cðr; t ! 1Þ A expðr=Þ þ M The inset shows the data in (b) where the r axis has been rescaled by t1=2 .

law Cðr; t ! 1Þ r at the critical point, with an exponential cutoff. The black dotted line shows that the exponent remains equal to 1=4 as argued in [21]. This value coincides with the exact result of the eight-vertex [4,23] and 2D Ising models. Note that the numerical data show clear signs of finite size effects when r L. In Fig. 4(b) we show the behavior of Cðr; tÞ after a quench into the c-AFM phase ( ¼ 1:36). As shown in [8,25], the approach to equilibrium is fast for a T ¼ 0 initial state, whereas it is very slow and occurs via a 1

1

20

40

week ending 17 MAY 2013

PHYSICAL REVIEW LETTERS

60

80

100 1

1

1

20

40

60

80

100

1

1

1

20

40

60

80

100 1

20

20

20

20

20

20

40

40

40

40

40

40

60

60

60

60

60

60

80

80

80

80

80

80

101

101 1

20

40

60

80

100

1

20

40

60

80

100

101 1

20

40

60

80

101 100

101 1

20

40

60

80

100

80

100 1

101

(a)

1

1

20

40

60

80

100 1

1

20

40

60

1

1

1

20

20

20

20

20

20

40

40

40

40

40

40

60

60

60

60

60

60

80

80

80

80

80

80

101 1

20

40

60

80

101 100

101 1

20

40

60

80

101 100

101 1

20

40

60

80

101 100

(b)

FIG. 5 (color online). Snapshots of L ¼ 102 samples at t ’ 102 , 103 , 104 MC simulations after a quench from ¼ 0 to the critical point, c ¼ 1:2 (a) and into the AFM phase, ¼ 1:36 (b). Pink regions (gray background) are c-AFM ordered; green points (clear gray) correspond to a, b-FM vertices; red and blue points (darker gray) correspond to oppositely charged defects of type e.

207206-4

PRL 110, 207206 (2013)

PHYSICAL REVIEW LETTERS

correlation functions). Another possibility is to analyze the spatial correlations. Indeed, the facility of imaging the microstates both numerically and experimentally makes such study very appealing. As an example, in Fig. 5 we show snapshots of microscopic configurations of L ¼ 102 systems after quenches from ¼ 0 to c ¼ 1:2 [Fig. 5(a)] and ¼ 1:36 [Fig. 5(b)]. The first two panels in each row are out of equilibrium while the last ones show typical equilibrium configurations at the critical point and inside the AFM phase, respectively, cf. Fig. 4. Large domains of AFM order form, separated by domain walls made by a and b vertices. These snapshots could be compared with MFM images of ASI configurations [19,20] at the corresponding values of (the experimental points closest to c ¼ 1:2 and ¼ 1:36 correspond to the samples produced using a Ti underlayer with lattice constants ‘ ¼ 466 nm and ‘ ¼ 433 nm, respectively). Conclusion.—In this Letter we studied the equilibrium and out-of-equilibrium properties of the 2D sixteen-vertex model using MC simulations and a sophisticated cluster variational Bethe-Peierls approach, and we compared our results to the recent experimental data on ASI [18–20]. We showed that the model describes with very good accuracy the behavior of the densities of the different vertex types of ASI samples obtained by gradual deposition of magnetic material on a square pattern as the lattice constant and the underlayer disorder are changed. This implies that the experimental samples of [19,20] are at—or at least very close to—thermal equilibrium. It is important to point out that our interpretation does not require any fitting parameter as the effective temperature introduced in [18,20]. We reveal the presence of a second-order phase transition from a conventional high temperature (large lattice constant, strong disorder) PM phase to a low temperature (small lattice constant, weak disorder) staggered AFM phase. Such a phase transition could hinder full equilibration, and should be unveiled by measuring long-range spatial correlations in the experiments. We close by insisting upon the fact that, although vertex models avoid all the complications of (long-range) dipolar interactions, they provide a very good schematic framework to study ASI from a theoretic perspective. The excitement around these samples as well as the intriguing excitation properties of spin ice (emergence of magnetic monopoles and attached Dirac strings [13] which have recently been observed in ASI [15,27]) should encourage their study from a novel and more phenomenological viewpoint. We thank T. Blanchard, C. Castelnovo, and C. Nisoli for very useful discussion and G. Brunell, J. Morgan, and C. Morrows for lending their experimental data to us. We acknowledge financial support from ANR-BLAN-0346 (FAMOUS).

week ending 17 MAY 2013

[1] L. Balents, Nature (London) 464, 199 (2010). [2] R. Moessner and A. P. Ramı´rez, Phys. Today, No. 2, 59, 24 (2006). [3] L. D. C. Jaubert, J. T. Chalker, P. C. W. Holdsworth, and R. Moessner, Phys. Rev. Lett. 100, 067207 (2008). [4] E. H. Lieb and F. Y. Wu, in Phase Transitions and Critical Phenomena, edited by C. Domb and J. L. Lebowitz (Academic, New York, 1972), Vol. 1, Chap. 8, p. 331. [5] R. Youngblood, J. D. Axe, and B. M. McCoy, Phys. Rev. B 21, 5212 (1980). [6] C. Henley, Annu. Rev. Condens. Matter Phys. 1, 179 (2010). [7] T. Fennell, O. A. Petrenko, B. Fa˚k, J. S. Gardner, S. T. Bramwell, and B. Ouladdiaf, Phys. Rev. B 72, 224411 (2005). [8] D. Levis and L. F. Cugliandolo, Europhys. Lett. 97, 30 002 (2012). [9] M. J. Harris, S. T. Bramwell, D. F. McMorrow, T. Zeiske, and K. W. Godfrey, Phys. Rev. Lett. 79, 2554 (1997). [10] S. T. Bramwell and M. J. Gingras, Science 294, 1495 (2001). [11] S. T. Bramwell et al., in Frustrated Spin Systems, edited by H. T. Diep (World Scientific, Singapore, 2004), Chap. 7. [12] A. P. Ramirez, A. Hayashi, R. J. Cava, R. Siddharthan, and B. S. Shastry, Nature (London) 399, 333 (1999). [13] C. Castelnovo, R. Moessner, and S. L. Sondhi, Nature (London) 451, 42 (2008). [14] R. F. Wang et al., Nature (London) 439, 303 (2006). [15] E. Mengotti, L. J. Heyderman, A. Fraile Rodrı´guez, F. Nolting, R. V. Hu¨gli, and H.-B. Braun, Nat. Phys. 7, 68 (2010). [16] C. Phatak, A. K. Petford-Long, O. Heinonen, M. Tanase, and M. De Graef, Phys. Rev. B 83, 174431 (2011). [17] G. Mo¨ller and R. Moessner, Phys. Rev. Lett. 96, 237202 (2006). [18] C. Nisoli, J. Li, X. Ke, D. Garand, P. Schiffer, and V. H. Crespi, Phys. Rev. Lett. 105, 047205 (2010). [19] J. P. Morgan, A. Stein, S. Langridge, and C. H. Marrows, Nat. Phys. 7, 75 (2010). [20] J. P. Morgan, J. Akerman, A. Stein, C. Phatak, R. M. L. Evans, S. Langridge, and C. H. Marrows, Phys. Rev. B 87, 024405 (2013). [21] L. Foini, D. Levis, M. Tarzia, and L. F. Cugliandolo, J. Stat. Mech. (2013) P02026. [22] E. V. Albano, M. A. Bab, G. Baglietto, R. A. Borzi, T. S. Grigera, E. S. Loscar, D. E. Rodriguez, M. L. Rubio Puzzo, and G. P. Saracco, Rep. Prog. Phys. 74, 026501 (2011). [23] R. J. Baxter, Exactly Solved Models in Statistical Mechanics (Dover, New York, 1982), Vol. 9. [24] R. C. Silva, F. S. Nascimento, L. A. S. Mo´l, W. A. MouraMelo, and A. R. Pereira, New J. Phys. 14, 015008 (2012). [25] Z. Budrikis, P. Politi, and R. L. Stamps, J. Appl. Phys. 111, 07E109 (2012). [26] A. J. Bray, Adv. Phys. 43, 357 (1994). [27] S. Ladak, D. E. Read, G. K. Perkins, L. F. Cohen, and W. R. Branford, Nat. Phys. 6, 359 (2010).

207206-5